We have shown that the transverse magnetoresistivity inside the hidden-order phase
of URu_{2}Si_{2} strongly depends on the sample quality. In fact, the orbital effect is
en-hanced when the mobility, proportional to the relaxation time (see Sect. 2.4), of the
charge carriers is higher. The relaxation timeτ increases with the purity of the
sam-ples and decreases with the temperature. An almost perfect compensation of
elec-trons and holes in URu_{2}Si_{2}is shown by the monotonously-increasing transverse
mag-netoresistivity in fields µ_{0}H∥aup to 80 T (see Fig. 7.2). Assuming that the
elec-tronic properties can be described by a unique relaxation time and an average
mobil-ity for all conduction bands, the magnetoresistivmobil-ity ∆ρ_{x,x}=ρ_{x,x}(H)−ρ^{n}_{x,x}(H = 0)
of a compensated metal with spherical Fermi surfaces is given by (see Sect. 2.4):

∆ρ_{x,x}

ρ^{n}_{x,x}(H= 0) = (ωcτ)^{2} =µ^{2}(µ0H)^{2}, (7.1)
whereρ^{n}_{x,x} is the zero-field resistivity estimated for the normal non-superconducting
state (virtual normal state at temperatures below T_{SC}, see Sect. 3.5).

7.4 Analysis of the magnetoresistivity
T = 100 mK and (b)T = 1.4 K. The scattered lines representH^{2}-dependencies.

∆ρx,x/ρ^{n}_{x,x}(H = 0) of samples (c) #1 and (d) #2 versus (µ0H)^{2} in µ0H∥ c
up to 20 T, at temperatures from 100 mK to 6 K.

Kasahara et al. [Kasahara 2007] have found, for a high-quality sample [RRR^{∗} =
ρ_{x,x}(300 K)/ρ_{x,x}(T → 0) = 670], a nearly perfect ∝ H^{2}-dependence of ∆ρ_{x,x} in
magnetic fieldsµ_{0}H∥c up to 10 T and Levallois et al. [Levallois 2009] have found
for a sample of lower quality [RRR =ρx,x(300K)/ρx,x(2K) = 40], a field-dependence
of ∆ρ_{x,x} close to ∝ H^{2} in fields H ∥ c up to µ_{0}H = 20 T. The resistivity of our
high-quality URu_{2}Si_{2} sample #2 increases by more than two orders of magnitude
in magnetic fields applied along a and c, as shown in Figures 7.2(a) and 7.3(a),
respectively. This exceptionally-strong transverse magnetoresistivity is due to a
very low carrier density [Levallois 2009] combined with the high sample-qualities
[Kasahara 2007, Matsuda 2011].

Figure 7.6 shows plots of the magnetoresistivity of samples #1 and #2 versus H^{2}
for µ_{0}H ∥ c up to 20 T at different temperatures from 100 mK to 6 K. The plots
show aH^{2}-dependence ofρ_{x,x} in low fields between∼3 and 13 T in agreement with

7 Orbital Magnetoresistivity
Levallois et al. (RRR = 40) [Levallois 2009]. The mobilities were extracted
from by the slope ofρ(H) versus (µ0H)^{2} in H∥c[see Fig. 7.6]. The dashed
lines are guides to the eyes. Mobility µ of samples #1 and #2 versus (c) T
and (d) 1/ρ^{n}_{x,x}(H = 0). The dashed lines are guides to the eyes.

the results of Kasahara et al. [Kasahara 2007] and Levallois et al. [Levallois 2009].

On the other hand, the behavior of the magnetoresistivity clearly deviates from
the H^{2}-dependence at higher fields. As the maximum in the resistivity at ∼30 T
[see Fig. 7.3(a)], the slope of the low-field H^{2}-dependence is enhanced with the
sample quality. I extracted a mobility µ averaged over all bands by fitting ρ_{xx}
versus H^{2}, in the regime between 3 and 13 T, using Equation (7.1). I note here,
that for temperatures below T_{SC} = 1.5 K, the zero-field resistivity ρ^{n}_{x,x}(H = 0) of
the normal non-superconducting state was obtained by the extrapolation via a fit
ρ_{x,x}(T) = ρ_{0} +AT^{1.5} to the resistivity between 1.5 and 8 K (see Sect. 3.5 and
[Matsuda 2011]). I found similar RRR-dependencies of the resistivity maximum at
H_{ρ,max}^{LT} [see Fig. 7.7(a)] and of the mobility [see Fig. 7.7(b)], both being strongly
enhanced with a higher sample quality. Figure 7.7(c) shows the mobility µ versus

7.4 Analysis of the magnetoresistivity
the temperature T extracted for samples #1 (RRR = 90) and #2 (RRR = 225)
inH∥c. The mobility is enhanced as the temperature decreases and a saturation
occurs due to a finite relaxation time in the limit of zero temperature (non-perfect
crystals). Figure 7.7(d) shows that the mobilitiesµof samples #1 and #2 increase
approximately linearly with 1/ρ^{n}_{x,x}(H= 0), which is compatible with the picture of
an isotrope metal with a unique relaxation time τ, where τ ∝1/ρ^{n}_{x,x}(H = 0) (see
Sect. 2.4).

The Kohler’s rule [Kohler 1938] implies that all plots of ∆ρ_{x,x}(H)/ρ^{n}_{x,x}(H = 0)
versus [µ0H/ρ^{n}_{x,x}(H = 0)]^{2} fall on a unique curve, which is independent of the
sample quality and the temperature (see Sect. 2.4.4). Levalloiset al. [Levallois 2009]

have shown that the Kohler plots from the resistivity of their sample (RRR = 40)
at temperatures between 1.5 and 17 K in fields µ0H ∥ c up to 20 T fall on a
same [µ_{0}H/ρ^{n}_{x,x}(H = 0)]^{2}-line. Figures 7.8(a) and (b) show the Kohler plots of the
resistivities of our samples #1 and #2, respectively, in fieldsµ_{0}H ∥ c up to 20 T,
at temperatures from 100 mK to 6 K. For sample #1, the plots coincide almost
up to 20 T and a H^{2}-dependence is clearly observed. For sample #2, the plots
coincide in a smaller field window (up to∼10 T) and deviate faster in higher fields
from theH^{2}-dependence than for sample #1. Figures 7.8(c) and (d) show the same
plots forµ_{0}H up to 40 T in a double-logarithmic scale. These plots emphasize that
the magnetoresistivity behavior changes drastically at low fields in the proximity
of H_{c2} and at the field-induced crossoversH^{∗} and H_{ρ,max}^{LT} . The deviation from the
H^{2}-dependence at low fields is due to the combination of the proximity ofH_{c2} and a
parasitic off-set in the raw resistivity data. Figures 7.8(e) and (f) compare the Kohler
plots of the resistivities of samples #1 and #2 and that from the sample studied
by Levallois et al. [Levallois 2009] in a double-logarithmic scale, at T = 100 mK
andT = 1.4 K, respectively. The plots of the different samples are close but do not
coincide in the low-field regime.

To summarize, the low-field magnetoresistivity exhibits aH^{2}-behavior, as predicted
for a metal with a compensated spherical Fermi surface (cf. also [Pippard 1989,
Kasahara 2007, Levallois 2009]). The extracted mobility depends on the sample
quality and the temperature. On the other hand, the high-field
magnetoresistiv-ity ∆ρ(H)/ρ(H = 0) deviates strongly from the H^{2}-behavior, namely, when
field-induced crossover-like anomalies in the magnetoresistivity occur atµ0H^{∗} ∼20−25 T
and µ_{0}H_{ρ,max}^{LT} ∼ 30 T. In fact, URu_{2}Si_{2} has a complex multi-band structure (see
Sect. 9.1) and field-induced Fermi surface modifications have been observed in
mag-netic fields far below the destruction of the hidden-order phase atµ0H1= 35 T (see
Sect. 9.2). ForH∥a, I could not analyze the magnetoresistivity, as done forH∥c,
because of a lack of reproducibility between the different sets of data (cf. Sect 3.9).

7 Orbital Magnetoresistivity

[Lev allois et al.]

sample
double-logarithmic scale. The scattered lines representH^{2}-dependencies.

7.4 Analysis of the magnetoresistivity For H∥a, the slope of the low-field magnetoresistivity is stronger and indicates a mobility higher than forH∥c [see also Chapt. 8, Fig. 8.4(b)]. Since the mobility is inversely proportional to the cyclotron effective mass (see Sect. 2.4), a higher mobility forH∥athan forH∥cis compatible with the anisotropy of the cyclotron effective masses extracted by Shubnikov-de Haas experiments [Aoki 2012].

### 8 Angle-Dependent Study of the High-Field Magnetoresistivity

URu2Si2 exhibits strongly anisotropic bulk properties due to the Ising-character
of its magnetic properties. The magnetic easy axis is the c-axis of the
body-centered tetragonal lattice. This results in strongly anisotropic
re-sistivity [Palstra 1986, Ohkuni 1997] and magnetic susceptibility [Palstra 1985,
Dawson 1989, Ramirez 1992]. The upper critical field H_{c2} related to the
destruc-tion of superconductivity is also strongly anisotropic [Kwok 1990, Brison 1994,
Ohkuni 1997]. Magnetization [Sugiyama 1990] and magnetoresistivity [Jo 2007]

measurements have shown that the low-temperature critical fieldsH_{1}, H_{2}, and H_{3}
follow a simple 1/cosθ-law, at least up toθ= 30^{◦}, whereθis the angle between the
magnetic field and the c-axis. Furthermore, Aoki et al. [Aoki 2012] observed that
the crossover field H^{∗} in the magnetoresistivity also follows a 1/cosθ-law, at least
up to θ= 30^{◦}. In this chapter, I present magnetoresistivity experiments performed
on the URu_{2}Si_{2} monocrystalline samples #1 and #2 in a rotation probe, which
per-mitted to measure the magnetoresistivity versus a magnetic field up to 60 T applied
along different orientations of the crystal. The basic crystal planes (a,c) and (a,c)
of the tetragonal structure have been investigated. These experiments extended the
angle-dependence of the transition fields H_{1}, H_{2}, and H_{3} and the crossover fields
H^{∗} and H_{ρ,max}^{LT} up to θ= 60^{◦}.

### 8.1 Angle dependence of H

_{c2}

Figure 8.1(a) presents the transverse magnetoresistivity ρx,x of our sample #2 of
URu_{2}Si_{2}versus the magnetic fieldHapplied parallel to the (a,c)-plane, for different
angles θ between the magnetic field and the c-axis at T = 32 mK. The resistivity
equals zero below the superconducting critical fieldHc2 and increases monotonically
above H_{c2}. The critical field µ_{0}H_{c2} equals 3.1 T for θ = 5^{◦} and increases with θ,
reaching 7.1 T for θ = 67^{◦}. In the normal conducting state, ρ_{x,x}(H) exhibits an
oscillatory modulation due to the Shubnikov-de Haas effect, which will be analyzed
in Chapter 9. The θ-dependence ofH_{c2} obtained by our resistivity experiments on
sample #2 is plotted in Figure 8.1(b). H_{c2} exhibits a pronounced anisotropy in the

8 Angle-Dependent Study of the High-Field Magnetoresistivity

Figure 8.1: (a) Magnetoresistivityρx,x of URu^{2}Si^{2}sample #2 versus the magnetic fieldH
for different anglesθbetweenHandcatT = 32 mK. (b) Angle-dependence of
Hc2 forHin the plane (a,c) from our resistivity data of sample #2 and from
resistivity data from [Ohkuni 1999]. ^{∗}The solid lines represent fits to the data
with the function (8.1).

(a,c)-plane. The angle dependence ofH_{c,2} obtained by Ohkuniet al. [Ohkuni 1999]

on another sample, also plotted in Fig. 8.1(b), is in good agreement with that from
our data. The data of Ohkuni et al. [Ohkuni 1999] show that, at T = 30 mK,
µ_{0}H_{c2} reaches ≃ 13 T for H ∥ a (θ = 90^{◦}). The angle dependence of H_{c,2} was
first established by Brison et al. [Brison 1994] from specific heat measurements.

They proposed a theoretical model for the anisotropy of H_{c2}, based on the Pauli
paramagnetic limit:

H_{c2}(θ) = H_{c2}(H∥c)

√cos^{2}(θ) +ϵ^{2}sin^{2}(θ), (8.1)
where ϵ = H_{c2}(H ∥ c)/H_{c2}(H ∥ a), and found that this model fits well to their
data at T = 10 mK. The angle-dependencies of Hc,2 established by Ohkuni et al.

[Ohkuni 1999] and in this work are well described by this model, too [see Fig. 8.1(b)].